Application of lentil seed extract as an inhibitor to assess the corrosion properties of copper–nickel alloys in a NaCl environment

Weight loss (WL), electrochemical, and surface analysis were used to explore the efficiency of lentil seed extract (LSE) in mitigating the electrochemical corrosion of Cu–10Ni and Cu–30Ni alloys in obviously aerated water. The adsorption of lentil seed extract (LSE) species to create a barrier layer improved the corrosion resistance of Cu–Ni alloys in a NaCl medium. It was shown that the temperature of the medium and the amount of extract used affected the enhanced inhibitory efficacy. Using the PDP approach, the Cu–10Ni alloy showed the maximum inhibition performance (IE) of about 98.58% and 8.53% with 300 ppm LSE, respectively. According to the findings, the studied extract had a good ability to slow down the step at which alloys corroded in a 3.5% NaCl solution. It was discovered that as the temperature rose, the rate of corrosion increased. The thermodynamic activation functions of the dissolution process were also calculated as a function of extract dose. PDP curve analysis reveals that LSE is a mixed-type inhibitor, and EIS findings demonstrates that increasing dose not only alters the charge transfer (Rct) of Cu–10Ni alloy from 1031 to 2984 Ω cm2 and for Cu–N30Ni alloy from 3093–6208 Ω cm2 but also changes the capacitance of the adsorbed double layer (Cdl) for Cu–10Ni alloy from 728–678 μF cm2 and for Cu–30 Ni alloy from 726 to 701 μF cm2. The inhibitor's adsorption provides a good fit for the “Freundlich, Temkin, and Langmuir isotherm” models. Several methods are used to confirm that the alloy surface has a protective coating.


Introduction
2][3][4] The protective layer that primarily consists of an inner barrier layer with noticeable amounts of oxygen, copper, and some nickel as well as a thick outer layer primarily composed of cuprous chloride is responsible for the corrosion opposition of Cu-Ni alloys.The alloy has outstanding resistance to corrosion because of its inner layer. 5owever, aer a prolonged exposure period, signicant corrosion invariably manifests itself in either hydrodynamic or calm conditions. 68][9] The economy is greatly impacted by corrosion, which affects "infrastructure, transportation, utilities, production, and manufacturing".1][12][13] In order to prevent corrosion on metals and alloys, organic compound-based corrosion inhibitors are frequently employed.
The majority of these substances, however, are synthetic chemicals that can be very costly, poisonous, and dangerous for the environment and living things.As a result, one of the essential procedures that should be modied to safeguard metals and composites from damage in a variety of industrial settings is the employment of environmentally friendly inhibitors.5][16][17][18][19] These extracts are entirely soluble in aqueous media, nontoxic, and reasonably priced.One of the most signicant metallic corrosion inhibitors is plant extract.They are renewable, easily accessible, harmless, safe for the environment, biodegradable, and very effective.The various plant sections that can be extracted are signicant since they contain a wealth of chemical compounds. 20,21These compounds can be easily and affordably extracted using simple techniques.3][24][25][26][27] Chieb, et al. 28 investigated the adsorption and inhibitory efficiency of acrylonitrile derivatives by means of a range of electrochemical methods.These techniques included: (E)-2(3-carbonyl 1-indole-3-)-3-(2-oxo-2-phenylethylthio)3H-indole-3carbonyl-3-(phenylamino)acrylonitrile (a), ((E)-2-b) and (Z)-3-mercapto-3-(phenylamino)acrylonitrile-2-(carbonyl-3-indole)-3 phenyl acrylonitrile (c) in 0.5 M HCl on the Cu10Ni alloy.The percentage of IE was 95.1%, 92.1%, and 90.4% for (a), (b), and (c), in that order.The effects of "3-methyl 4-amino 1,2,4 triazole on the oxidization behavior of Cu-Ni 70-30 (Monel) in a 3% NaCl solution at 25 °C are evaluated by Deyab et al. 29 At 60 ppm, the inhibitor (MATA) reached its maximum percentage of IE (95%) and the inhibitor's efficacy decreased with increasing dose.Aesculus Hippocastanum Seeds (AHS) extract was employed by Loto et al. 30 as a corrosion inhibitor to lower the danger of copper alloy corrosion during the acid cleaning (5 N H 3 PO 4 ) process in desalination facilities.The ndings indicated that the AHS extract has a 96.1% inhibitory efficiency as a corrosion inhibitor at 100 ppm.The study conducted by Li et al. 31 examined the effects of admixing 1 : 1 "Citrus paradisi and Cymbopogon distillates on Cu-Ni alloy in 0.25 M H 2 SO 4 -3.5% NaCl electrolyte".The results showed that the Cu-Ni alloy degradation rate without distillate is 0.373 mm per year, while at 1% dose, the degradation rate decreased to 0.140 mm per year (1.37 × 10 −5 A cm −2 ), indicating an inhibition efficiency of 62.46%.Inhibition efficiency varied from 80.47 to 95.58% at a dosage of 2-5 percent.In a 3.5% sodium chloride solution, the corrosion inhibition behavior of methionine (Met), an environmentally benecial amino acid, and its synergistic effect with sodium silicate (SS) for copper-nickel alloy (Cu-10Ni) were studied. 32ccording to the ndings, Met has the best inhibitive efficacy of any cathode corrosion inhibitor, measuring 62% at an additional concentration of 40 ppm.Due to the synergistic action of two corrosion inhibitors, a compact and uniform layer forms on the surface of the cupronickel specimen when 20 ppm met and 20 ppm SS are added concurrently, increasing the inhibitive efficiency to 90%.In a corrosive solution containing 6% HCl with ethylenediamine (EDA) and tetraethylenepentamine (TEPA) as corrosion inhibitors, Mohamed et al. 33 investigate the effects of temperature and inhibitor dosage on the corrosion of a copper-nickel alloy.At 40 °C, the highest % IE for TEPA and EDA was determined to be 56.3% and 77%, respectively.The efficiency of inhibition increases with an increase in inhibitor dose and declines with an increase in temperature.Green tea aqueous extract is used as a durable corrosion inhibitor for two Cu-Ni alloys in 3.5% NaCl, according to Gaber et al. 34 The capabilities of protable freshening water (lime water) were compared with this one.The results show that the extract under test was able to effectively slow down the rate at which alloys rusted in 3.5% NaCl.In sulde-polluted salt water, Cu10Ni alloys electrochemical and SCC characteristics are investigated by Abd El-Nazeer et al. 35 Additionally, they evaluate how glycine (gly) affects the Cu10Ni alloy's susceptibility to SCC in these media and investigate any possible synergistic effects between gly and KI on the effectiveness of erosion inhibition.The maximum efficiency is 87.32% in the presence of KI and 80.54% in the free KI solution.
This paper aims to assess the inhibitory effect of LSE on Cu-Ni alloys corrosion in a 3.5% NaCl solution.WL, PDP, EIS, EFM, and surface morphology experiments were used to conrm the LSE corrosive inhibition.Data on kinetics and thermodynamics were also assessed.

Materials and solutions
The chemical makeup (wt%) of the two kinds of copper-nickel alloys employed in this investigation is as follows: 1.67 Fe, 0.768 Mn, 9.27 Ni, and a balance of Cu were found in the Cu-10Ni alloy, whereas 0.02 Fe, 0.44 Si, 0.51 Ca, 29.16 Ni, and a balance of Cu were found in the Cu-30Ni alloy."Prior to each experiment, the working electrode was polished with SiC, rinsed with ethanol and nally with doubly distilled water"."The auxiliary electrode was platinum wire, while a reference electrode calomel electrode (SCE), connected to a conventional electrolytic cell of capacity 100 mL".The experiments were studied the corrosion behavior of two of Cu-Ni alloys in 3.5% NaCl solution in the absence and presence of different dose of LSE as a natural product (50, 100, 200, and 300 ppm)."All solutions were freshly prepared using analytical grade reagents and doubly distilled water".The corrosion inhibition of Cu-Ni alloys in 3.5% NaCl solution, which has a salt content similar to seawater, was assessed using chemical and electrochemical methods in the absence and presence of various dosages of LSE as a naturally occurring product.

Preparation of plant extracts
Different parts of the selected plants were collected from various regions of Daqahlia Governorate January 2023.These included leaves, bark and roots of lentils.The plant was iden-tied at the Botanical herbarium at Sadat City University.Each plant sample was air dried and ground into a ne powder by used an electrical mill.Methanol is known to be powerful extraction solvent of compounds from plants. 36Therefore, two hundred grams (200 g) of this powder was soaked in 800 mL of methanol, at a ratio of 1 : 4 (powder/solvent) for 48 h at room temperature.Under vacuum the extract was removed and dried by rotary evaporator. 37The extract was then concentrated at 68 °C under reduced pressure to obtain the residues that constituted the crude extract.The investigated extract was liqueed in ethanol (1 g L −1 ) and conserve into refrigerator.All of the extracts were kept at 4 °C until further use.The main chemical structure existing in lentils extract before and aer study of the corrosion inhibition are represented below (Scheme 1).

Weight loss (WL) measurements
The WL approach is the simplest way to evaluate corrosion losses.The samples are rst properly cleaned, aer which they are polished with different grades of SiC, washed in ethanol, rinsed in doubly distilled H 2 O, and then allowed to dry.Following these stages, the specimens were precisely weighed before being submerged in 100 mL of 3.5% NaCl in both the attendance and lack of LSE natural products (50, 100, 200, and 300 ppm).At a temperature of 25 °C, WL measurements were collected over 15 days.The specimens were removed from the test solution, completely cleaned of corrosion products, and then allowed to dry before being precisely reweighed."Triplicate samples were used to check reproducibility of results".Eqn (1) & (2) (ref.38) can be used to get the average WL in grams and the corrosion rate (CR), respectively: This is how the corrosion rate (CR): is calculated where T is the immersion duration in days, A is the Cu-Ni electrode's area in cm 2 , DW is the WL in kg, D is the electrode's density in grams per cube centimeter, and k is a constant (8.76 × 10 4 ).Eqn (3) yields the inhibition efficiency (% IE) and surface coverage (q).
where CR o and CR inh are the corrosion rates of the alloys in the absence and existence of LSE, respectively.
where i corr(inh) and (i corr(free) ) are the corrosion current density in presence and absence of the extract, respectively.

EIS tests.
Using ac signals at open circuit potential, EIS of Cu-Ni alloys was performed in the frequency range of 100 kHz to 10 mHz with an amplitude of 10 mV peak-to-peak.The following eqn (5) denes the q and the percentage IE that were received from the EIS 38 where R ct and R ct(inh) are the charge transfer resistance in the absence and presence of LSE, respectively.The main parameters deduced from the analysis of Nyquist diagram are the resistance of charge transfer R ct (diameter of high frequency loop) and the capacitance of double layer C dl .Since the electrochemical theory assumed that 1/R ct is directly proportional to the capacity of double layer.

Adsorption isotherm
The type of adsorption isotherm can reveal more details about the characteristics of the LSE under study.To get the adsorption isotherm, the extent of surface coverage (q) of the two Cu-Ni alloys by the LSE must be evaluated by diverse adsorption isotherms.In this investigation, the (q) for altered doses of the LSE in marine solution has been estimated from the WL, PDP, and EIS methods.

Spectroscopic analysis
We looked into the surface morphology of the two Cu-Ni alloys with and without LSE.The Cu-Ni alloys were polished and honed before being dipped into the electrolyte solutions.Following a 15-days immersion in NaCl solutions, SEM micrographs of the alloy's surface were acquired, both with and without the LSE under examination.In this work, the JEOL JSM model scanning electron microscope (SEM) at Mansoura University in Egypt was coupled with an energy dispersive spectroscopy (EDX).

Impact of LSE as corrosion inhibitor
% IE and CR values for "two Cu-Ni alloys" achieved by the method of WL at different doses of LSE are condensed in Table 1 and Fig. 1.As seen in presence of extract, the WL of the two alloys decreased.The CR becomes lower with increasing the dose of LSE.This action may be attributed to a competitive step, including passive lm healing by the extract and passive lm damage by the aggressive ions.The outcomes revealed that extract hinder the consumption of Cu-Ni alloys.% IE increments pointedly with increments in extract dose arriving at the most extreme estimation of 86.7% in presence of 300 ppm of extract for Cu-10Ni alloy and 73.5% for Cu-30Ni alloy.This conduct could be claried by the adsorption of segments of the extract on the surface of Cu-Ni alloys bringing about the hinder of the dissolution and protecting the surface in the corrosive medium.By increasing the dose of the extract in the corrosive solution, the effectiveness of inhibition was improved."As a result, a protective lm that is more durable and sticky forms on the surface". 39Thusly, we can infer that the LSE is a good inhibitor for Cu-Ni alloys in 3.5% NaCl solution.

Effect of immersion time
One crucial factor that can be used to assess the stability of inhibitor function is the immersion time. 40Fig. 2 shows how the WL of Cu-Ni alloys in 3.5% NaCl changes over time, both with and without varying the dose of LSE.The graph indicates that WL rises as the duration of contact time does.The dissolution rate of used alloys in 3.5% NaCl 41 reduces as the dose of LSE increases, suggesting that LSE slows down the rate of corrosion.The phytochemical ingredients included in LSE are responsible for the extract's inhibitory impact.The WL Fig. 1 The variation of dissolution rate on two "Cu-Ni alloys" in 3.5% NaCl with different doses of LSE at 298 K after 15 days immersion.Paper RSC Advances of Cu-Ni alloys was shown to rise with temperature at higher temperatures (plots not shown), indicating desorption of the adsorbed protective layer from the alloy surface at higher temperatures.

PDP measurements
The PDP study offers important information about the kinetics of the processes that take place at the anodic and cathodic regions as well as the kind of inhibition that corrosion inhibitors use based on corrosion potential.Fig. 3 displays the PDP curves for the two used alloys in a 3.5% NaCl solution with and without varying percentages of LSE.This gure makes it evident that the presence of LSE increased the anodic and cathodic overvoltage and caused a slight displacement in the Tafel lines, indicating that the extract acts as a mixed-type inhibitor by affecting the retardation of the two reactions (cathodic hydrogen reduction and anodic metal dissolution) without altering the dissolution mechanism. 42

EIS technique
EIS studies of the Cu-Ni alloys in the presence and absence of various dosages of LSE were conducted in order to learn more about the inhibitor process and to validate the results of the WL and PDP experiments.The Nyquist curve for the Cu-Ni alloys in a 3.5% NaCl solution, both in the absence and with varying dosages of LSE, is displayed in Fig. 4. Table 3 lists the EIS  parameters, capacitance double layer C dl , charge transfer resistance R ct , the q, and the percentage of IE.A depressed semicircle with the center under the real axis can be seen in the impedance spectra of Cu-Ni alloys in 3.5% NaCl.This type of behavior is typical of solid electrodes and is sometimes referred to as the frequency dispersion of interfacial EIS.The primary causes of this capacitance dispersion at the metal surface are the extract molecules' adsorption-desorption process on the surface of used alloys, surface roughness, and surface chemical heterogeneity. 44In order to address this, the equal circuit is modied to substitute a continual phase element (CPE) for C dl .CPEs are associated with surface roughness, contaminants, degree of polycrystallinity, chemical inhomogeneities, and adsorption inhibitive molecules. 45This is the impedance function, or CPE: 44 where n is the CPE exponent, which indicates the departure from the ideal performance and runs from 0 to 1, Y 0 is the CPE constant, j is the imaginary unit, and u is the angular frequency.The reduced value of n (Table 3) for Cu-Ni alloys in the investigated corrosive solution denotes surface irregularities brought on by corrosion-induced surface roughening of the alloys.The adsorption of extract molecules on the metal surface decreases its electrical capacity because they displace the water molecules and other ions originally adsorbed on the metal surface.This modication results in an increase of charge transfer resistance R ct which "suggest the formation of a protective layer on the Cu-Ni alloys surface".This layer makes a barrier for mass and charge transfer."The data in Table 3 show that the R ct increases with the increase in the extract dose in 3.5% NaCl solution, indicating a marked anticorrosion effect of the LSE on Cu-Ni dissolution in 3.5% NaCl solution".The reciprocal of R ct , is directly proportional to the corrosion current density and corrosion rate. 46This means that the corrosion rate decreases with increasing the extract dose."Also, the data in Table 3, show that the C dl and Y 0 values were almost decreased with the increase of the dose of investigated extract in 3.5% NaCl solution"."Y 0 for the blank is estimated to be higher than Y 0 for the inhibited solution; this suggests that the extract molecules interacted with the electrode surface, minimizing the erosion of the electrode's exposed locations".The decrease in C dl , which can result from a decrease in local dielectric constant and/or an increase in the thickness of the electrical double layer, suggests that LSE act by adsorption on the alloy/solution interface.The tted results show excellent agreement with the experimental data, as indicated by the small chi-squared values (Table 3) obtained for each result.The accuracy of the tting ndings was evaluated using the chisquared.Fig. 5 depicts the equivalent circuit that was utilized to duplicate the EIS data.Since this circuit uses CPE rather than capacitors to provide multiple forms of non-homogeneity, such as corrosive electrode surface roughness, grain boundaries, and alloy surface imperfections, we choose to employ it.The % IE calculated from EIS data are closed to those obtained from WL and PDP.The results showed the good agreement between measurements obtained from all techniques.In all measurements the % IE of Cu-30Ni alloy is greater than its in Cu-10Ni alloy at all doses of LSE, this is due to the increase of Ni content of Cu-Ni alloys in chloride solutions improve the corrosion resistance of these alloys 47

Adsorption isotherms
Using eqn ( 3) & ( 4), the surface coverage (q) and inhibitory efficiency (% IE) are determined based on the measurements of WL, PDP, and EIS.A number of adsorption isotherms, including Langmuir, Temkin, and Freundlich, were tted to the data in order to analyze them.
3.5.1 Langmuir adsorption isotherm.Using an appropriate tting of the adsorption isotherm, the values of (q) were graphically calculated from various techniques to examine the extract's adsorption process on the surface of Cu-Ni alloys.Using the following equation, the best connection was derived from the Langmuir adsorption isotherm: 48 The inhibitor adsorption equilibrium constant, K ads , is dened as follows: C represents the inhibitor dose.A plot matching the Langmuir adsorption isotherm is shown in Fig. 6, with C/q as the X-axis and C as the Y-axis.For Cu-10Ni and Cu30Ni alloys, respectively, a perfect linear curve was generated with regression constants R 2 > 0.9982 and > 0.9973.The equilibrium constant of the inhibitor's adsorption is oen related to DG ads .It might be calculated using eqn (8): 48 K ads = 1/55.5exp(−(DG ads /RT)) where 55.5 was the molar dose value of water in solution in mol dm −3 , R is the gas constant, T is the absolute temperature, and   DG ads is dened as the standard free energy of inhibitor adsorption.Table 4 presents the calculated standard Gibbs free energy of adsorption of the extract at 298 K.When the values of DG ads are around −20 kJ mol −1 or lower, the adsorption is due to the electrostatic interaction between the charged molecules of the extract and the charged electrode (physisorption).Meanwhile, those more negative than −40 kJ mol −1 reveal the charge transfer from the extract to the surface of the alloys to form a coordination bond (chemisorption) 49 In this current work, the obtained negative values of DG ads (less negative than  5 & 6, respectively.[52] where E * a is the activation energy, R is the gas constant, A is the pre-exponential factor of Arrhenius.5 and 6 It is clear from the Table 5 that, I corr decreases with increasing doses of LSE and hence % IE increases, on other hand, in Table 6 I corr , for used alloys, increases with increasing temperature, and hence lowering in % IE.Fig. 9 represents the Arrhenius plots of the Ln CR vs. 1/T for the used alloys in 3.5% NaCl with and without 300 ppm LSE at various temperatures.From the slopes of these plots -E * a =R; the activation energy ðE * a Þ values were calculated.The calculated E * a values and regression coefficient of Cu-10Ni alloy in 3.5% NaCl with 300 ppm LSE were 34.47 kJ mol −1 and 19.83 kJ mol −1 , 0.9458, and 0.9653, respectively, while for the Cu-30Ni alloy were 14.43 kJ mol −1 , 6.77 kJ mol −1 , and 0.9790, 9653, respectively.Arrhenius indicates that the faster the dependence of the CR with the temperature the higher E * a . 53"It is noticed that the formation of adsorbed lm on the surface of the alloys with increasing thickness that decrease the dissolution of used alloys".The increase values of E * a with LSE than in its absence for the two alloys indicate the physical adsorption of LSE on alloys surface.attacking the electrode surface, causing surface corrosion"."On the other hand, in the presence of LSE, less destruction was observed in the micrographs of the electrodes"."These results conrm that the surface has greatly enhanced, with a valuable and observable reduction in the corrosion rate"."This improvement is owing to the creation of a good protective layer on the used alloys surface from the LSE, which prevents the corrosion"."EDX spectra of the two used alloys are shown" in Fig. 11.This gure showed that the elements present on the surface of Cu-Ni alloys.Table 7 depicted the EDX spectrum results of the Cu-Ni alloys specimen for elemental composition with and without extract.This reveals that the predominant species, which is found on the electrodes surface, is form an adsorbed protective layer on alloys surface.The EDX analysis of the surface in the presence of LSE showed the presence of oxygen along with the reduction of the chloride signal.This is possibly due to the adsorption of LSE via oxygen active centers on the Cu-Ni alloys surface".In addition, the less porous property of the inhibitor-covered surface resulted in less penetration of the chloride ions onto the used alloys.Ni alloys surface that was exposed to a 3.5% NaCl solution but was not treated with the LSE was substantially greater at 300 nm and for Cu-30Ni alloy equal 400 nm.The acid's corrosive effects over the course of 3 hours rust test period le the alloys surface with a porous structure and deep fractures, which led to this heightened roughness.However, when the tested inhibitors are applied at the optimum dose (300 ppm LSE), the average roughness for Cu-10Ni alloy & Cu-30Ni alloy is reduced to 98 & 110 nm, respectively.The test LSE effectively maintain hardness of Cu-Ni alloys, as seen by the drop in roughness value. 54,55

The proposed adsorption mechanism of the extract
The adsorption of an inhibitor depends on its chemical structure, its molecular size, the nature and charged surface of the metal, and distribution of charge over the whole inhibitor molecule.In fact, adsorption process can occur through the replacement of solvent molecules from the metal surface by  ions and molecules accumulated near the metal/solution interface.Ions can accumulate at the metal/solution interface in excess of those required to balance the charge on the metal at the operating potential.These ions replace solvent molecules from the alloy surface, and their centers reside at the inner Helmholtz plane.This phenomenon is termed specic adsorption, contact adsorption.The anions are adsorbed when the alloy surface has an excess charge in an amount greater than that required to balance the charge corresponding to the applied potential.The exact nature of the interactions between the alloy surface and an aromatic molecule depends on the relative coordinating strength towards the given metal of the particular groups' present. 56Generally, two modes of adsorption were considered.In one mode, the neutral molecules of leaves extract can be adsorbed on the surface of alloy through the chemisorption mechanism, involving the displacement of water molecules from the alloy surface and the sharing electrons between the heteroatoms and Cu.The extract molecules can also adsorb on the alloy surface based on donor-acceptor interactions between p-electrons of the aromatic/heterocyclic ring and vacant d-orbitals of surface iron.Since all the different parts of plant extract possess several heteroatoms containing active constituents, therefore there may be a synergism between the molecules accounting for the good inhibition efficiencies.

Conclusions
From our experimental obtained values, the following conclusions can be made: (1).In 3.5% NaCl environment, lentil seed-methanol extract showed surface active characteristics and performed well as an inhibitor to stop Cu-Ni alloy corrosion.
(2) The PDP curves indicate that this LSE behaves as mixedtype inhibitor i.e.LSE reduces both cathodic and anodic corrosion in NaCl solution.
(3) According to the results of the WL measurement, LSE effectively inhibits the corrosion of Cu-Ni alloys in a 3.5% NaCl solution.(4) By increasing the temperature the % IE decreases, on the other hand, it dropped by increase the LSE dosages.
(5) The adsorption of LSE on Cu-Ni alloys surface is a physical one and obeyed, Langmuir, Temkin, and Freundlich models.(6) There is strong correlation between outcomes derived from the WL method and PDP, EIS techniques.

2. 4
Electrochemical tests 2.4.1 Potentiodynamic polarization (PDP) tests."PDP of the two Cu-Ni alloys were carried out at range of potential from (−800 to 300 mV) and scan rate 0.2 mV s −1 " in all solutions with and without LSE, then Tafel lines are plotted and the CR without (CR o ) and with (CR inh ) extract, corrosion potential (E corr ) values were recorded.The % IE and q are determined by eqn (4).

Scheme 1
Scheme 1 Chemical structures of lentils extract (a-f).
(20.4 to 25.9 mV) in the E corr values of inhibited systems compared to the uninhibited solution.The extract's ability to inhibit alloy oxidation and reduce hydrogen evolution is indicated by the tendency of E corr values to move in a positive direction.This suggests that the extract functions as a mixedtype corrosion inhibitor.

Fig. 2
Fig. 2 WL-time curves for used alloys dipped in 3.5% NaCl with and without different doses of LSE.

Fig. 3
Fig. 3 PDP curves for used alloys in 3.5% NaCl with and without altered doses of LSE.

Fig. 4
Fig. 4 Nyquist plot for used alloys in 3.5% NaCl solution in the absence and presence of different doses of LSE at 25 °C.

Fig. 5
Fig. 5 Electrical circuit model used to fit EIS results.
−20 kJ mol −1 ) show that the adsorption process of the extract on Cu-Ni alloys in 3.5% NaCl solution is spontaneous, also indicates the stability of adsorbed layer on Cu-Ni alloys surface and the adsorption of the studied LSE follows physisorption.The Temkin and Freundlich isotherms data and gures are represented in Fig 1S and 2S.† 3.6 Impact of temperature on inhibition process By using PDP tests the effect of temperature on used alloys in 3.5% NaCl solution in lack and attendance of 300 ppm LSE was studied in the temperature extent (25-60 °C).The CR, I corr , E corr and Tafel constants of Cu-Ni alloys in 3.5% NaCl solution as a function of temperature in absence presence of 300 ppm of LSE are summarized in Tables

Fig. 6
Fig. 6 Langmuir isotherm plot for the corrosion of Cu-Ni alloys in 3.5% NaCl solution in the absence and presence of different doses of LSE at 25 °C.

Fig. 7 &
8 show the PDP curves for two used alloys in 3.5% NaCl solution in the absence and presence of 300 ppm LSE at altered temperatures, respectively.The electrochemical parameters such as E corr , I corr , anodic (b a ) and cathodic (b c ) Tafel slopes, and CR are tabulated in Tables

3. 7
Surface analysis 3.7.1 SEM/EDX investigation.Fig. 10 obviously illustrates the SEM images of Cu-Ni alloys exposed to 3.5% NaCl solution with and without LSE."The SEM images of the corroded Cu-Ni alloys aer submersing in 3.5% NaCl solution and which appeared as a rough surface with many cracks and pores"."This result is due to the Cl − ions in the medium aggressively

Fig. 7
Fig. 7 PDP curves for Cu-Ni alloys in 3.5% NaCl solution at different temperatures.

Fig. 8
Fig.8PDP plots for used alloys in 3.5% NaCl solution in attendance of 300 ppm LSE at altered temperatures.

Fig. 9 A
Fig. 9 A plot of Ln CR versus 1/T for Cu-Ni alloys in 3.5% NaCl containing 300 ppm LSE altered temperatures.

Fig. 10
Fig. 10 Surface morphology for Cu-Ni alloys exposed to 3.5% NaCl solution with inhibitor.

Fig. 11
Fig. 11 EDX spectra for the used alloys exposed to 3.5% NaCl with LSE.

Fig. 12
Fig. 12 Surface morphology for Cu-Ni alloys exposed to 3.5% NaCl solution with and without LSE.

Table 1 %
IE, CR, and q for "Cu-Ni alloys in 3.5% NaCl solution" with and without different doses of LSEs following 15 days of immersion © 2024 The Author(s).Published by the Royal Society of Chemistry RSC Adv., 2024, 14, 28044-28057 | 28047

Table 2
43ovide the electrochemical properties of the used alloys, including a percentage of IE and CR, "as well as corrosion potential, E corr , anodic Tafel slope b a , cathodic Tafel slope b c , and corrosion current density, I corr ".It is evident from these tables that I corr values fell as LSE dosages increased.Cang et al.43discovered similar behavior.According to Table2, there is a shi of <85 mV

Table 2
Corrosion parameters for used alloys in 3.5% NaCl solution with and without different doses of LSE

Table 3
EIS parameters for used alloys in 3.5% NaCl solution in the absence and presence of altered doses of LSE at 25 °C

Table 4
Collects the adsorption parameters for all mentioned adsorption isotherms that obtained from graphical representation

Table 5
Corrosion parameters for Cu-Ni alloys in 3.5% NaCl solution at different temperatures

Table 6
Corrosion parameters for used alloys in 3.5% NaCl solution in attendance of 300 ppm LSE at various temperatures

Table 7
EDX spectrum results of the Cu-Ni alloys specimen for elemental composition with and without extract